Download (direct link):
3.0 THERMAL PROPERTIES
The states of low molecular weight compounds are well known: crystalline, liquid and gaseous. By contrast, no high molecular weight polymer vaporizes to a gaseous state; all decompose before the boiling point. In addition, no high molecular weight polymer attains a totally crystalline structure, except in the very rare single crystal state. In fact, many important polymers do not crystallize at all but form glasses at low temperature. At higher temperature, they form rubbers. The transition that separates the glassy state from the
rubbery state is known as the glass-rubber, or glass transition. The glass transition temperature (Tg) is an indication of the glass-rubber transition.
Qualitatively, the glass transition region can be interpreted as the onset of long-range, coordinated molecular motion. While only 1-4 chain atoms are involved in motions below the glass transition temperature, some 5-10 chain atoms attain sufficient thermal energy to move in a coordinated manner in the glass transition region. f27l
There are a number of structural features which determine the value of the glass transition temperature. Since the glass transition temperature is a temperature at which molecular rotation about single bonds becomes restricted, it is obvious that these features are ones which influence the ease of rotation. Factors which affect the glass transition temperature are as follows: (i) groups attached to the backbone which increase the energy required for rotation; (ii) rigid structures, e.g., phenylene groups, incorporated in the backbone of the molecule; (Hi) secondary bonding between chains, e.g., hydrogen bonding; (iv) primary bonding between chains, e.g., crosslinking; (v) length of side chains; (vi) molecular weight, and (vii) plasticization.
Plasticization is very important in polymer processing. For example, low molecular weight compounds are added to poly(vinyl chloride) during its processing to separate (solvate) chains and increase their mobility. The effect of plasticization will cause a marked reduction in the glass transition temperature. The addition of about 40% of diethyl hexyl phthalate to poly(vinyl chloride) will reduce its glass transition temperature by about 100°C. As presented in Sec. 3.3, carbon dioxide can also plasticize polymers and cause a tremendous decrease in the glass transition temperature. On the other hand, the effect of plasticization may induce or increase crystallization during the outgas process of absorbed gases for those polymers which have the structural regularity.
An evaluation of the effect of high pressure carbon dioxide with three polymers (two amorphous and one semicrystalline) is presented. The properties studied include the glass transition temperature, the melting temperature, and the melting enthalpy.
3.2 Experimental Procedure
Three polymer sheets of poly(methyl methacrylate) (PMMA), polyethylene terephthalate glycol modified (PETG) and polyethylene terephthalate (PET) were used. These polymers are all transparent with thicknesses of 1.5, 1.0 and 0.26 mm, respectively. Couponshaped samples of 1 * 4 cm2 were made from all three polymers and subjected to carbon dioxide treatment at 3,000 psi and 25°C. The treatment was held for one hour and then the high pressure chamber was decompressed to atmospheric pressure over one additional hour. The carbon dioxide treated samples were immediately subjected to differential scanning calorimetry (DSC) and thermogravimetric analysis (TGA) evaluations. These treated samples were stored in clean PE bags at 23 ± 2°C for subsequent evaluations. DSC evaluation was performed to obtain the glass transition temperature (Tg), the melting temperature (Tm) and the melting enthalpy (AH) using a Perkin Elmer DSC-2C with a heating rate of 20°C/min for all three polymers. A Du Pont Model 2950 TGA was used to evaluate the total amount of carbon dioxide uptake in polymers. A constant heating rate of 20°C/ min was used for all thermogravimetric analyses.
3.3 Results and Discussion
PMMA and PETG both showed significant swelling with extensive bubble/foam formation in the bulk of the material when treated in carbon dioxide at 3,000 psi and 25°C for one hour with decompression to atmosphere taking one additional hour. PET however, showed no significant changes when treated under identical conditions. This is due to the crystalline nature of PET as compared to complete amorphous character of both the PMMA and PETG.
Thermogravimetric analysis (TGA) is an analytical technique for determining the weight change of a sample as a function of temperature and/or time. Figures 5 through 7 show representative thermogravimetric profiles for PMMA, PETG and PET, respectively, that had been treated with carbon dioxide. The weight losses in the range of about 120-150°C has been assigned to the outgassing of carbon dioxide from polymers while weight losses occurring in the